Copper Recovery from Barren Cyanide Solution by Using Electrocoagulation Iron Process

This paper is a brief overview of the role of inducing the nucleated electro winning of copper by using iron electrodes in electrocoagulation (EC) process. Cyanide compounds are widely used in gold ore processing plants in order to facilitate the extraction and subsequent concentration of the precious metal. Owing to cyanide solution employed in gold processing, effluents generated have high contents of free cyanide as well as copper cyanide complexes, which lend them a high degree of toxicity. In this regard, two options for the treatment of cyanide barren solutions has been used; in two ways; first for cyanide destruction by oxidation with the use of the EC process, in theory, has the advantage of decomposing cyanide at the anode and collecting copper simultaneously by a sludge of copper magnetic iron. In both cases excellent performance can be achieved using the high capacity of the bipolar iron EC technology. We found that it is possible to reduce the copper cyanide complex from 720 mg·l to below 10 mg·l within 20 minutes.


Introduction
Due to the dwindling resources of simple cyanide extractable gold deposits, a large proportion of the gold processed in the 21st century will be recovered from complex gold ores, many of which will contain soluble copper minerals.It has been estimated that about 20% of all gold deposits have significant copper mineralization commonly associated with chalcopyrite, tetrahedrite, tennantite, enargite as well as bornite and chalcocite in certain ores [1].It has also been found that the majority of copper minerals including copper oxides, carbonates, sulfides (with the exception of chalcopyrite) and native copper are highly soluble in cyanide solutions [2].These copper containing minerals are problematic because, when ores containing such minerals are leached with cyanide to recover the gold, copper also dissolves to form stable copper cyanide complexes.The dissolution of copper consumes a substantial quantity of cyanide and thus, if not recovered imposes a significant financial cost on the gold mine.The presence of copper also causes other problems such as competition with gold to adsorb on carbon unless a sufficient free cyanide concentration is maintained, depletion of gold electrowinning cell efficiency, and gold losses by cementation onto certain copper minerals.Ores containing greater than 0.5% reactive copper may be generally considered uneconomical to process via conventional cyanidation due to the high reagent cost.Therefore, it is necessary to reduce the amount of copper, especially in leaching circuits, in order to increases the dissolution of gold and silver, to achieve this goal it is possible to remove the copper from barren solution after Merril-Crowe process using the electrocoagulation process (EC).This process can be interesting for the copper cyanide removal from processed solutions after the Merrill Crowe process, also has low cost of operation and investment.

Copper Cyanide Chemistry
The major challenges to the processing of gold-copper ores using cyanidation is that of the high cyanide consumptions that are typically experienced, along with effective control of the leach, particularly when there is variable cyanide-soluble copper in the ore.It is widely accepted that gold dissolution in cyanide solutions occurs as sequence of two reactions shown in Equations ( 1) and (2), Elsner's equation shows that oxygen is critical for the dissolution of gold.
The stoichiometry of the process shows that 4 moles of cyanide are needed for each mole of oxygen present in solution.At room temperature and standard atmospheric pressure, approximately 8.2 mg of oxygen are present in one liter of water.This corresponds to 0.27 × 10 −3 mol/L accordingly, the sodium cyanide concentration (molecular weight of NaCN = 49) should be equal to 4 × 0.27 × 10 −3 × 49 = 0.05 g/L or approximately 0.01%.This was confirmed in practice at room temperature by a very dilute solution of NaCN of 0.01% -0.5% for ores, and for concentrates rich in gold and silver of 0.5% -5% [3].Also, lime is added to keep the system at an alkaline pH of 10.5 -11.0.Other factors affecting gold leaching kinetics are grain size, agitation speed, temperature, pressure, foreign ions and cyanicides.
Free cyanide exists as the uncomplexed cyanide ion, CN − , and molecular hydrogen cyanide, HCN.These species are related by the acid dissociation of HCN: The concentration of free cyanide is the sum of the CN − and HCN concentrations, and the equilibrium diagram shown in Figure 1 illustrates the distribution.
This figure shows the proportions of free cyanide as CN − , and HCN as a function of pH at 25˚C.At pH values below 7, cyanide is predominantly present as the unionized HCN molecule, which is easily volatilized because of its high vapor pressure.The equilibrium is displaced in favor of cyanide ion formation at pH values above 7. Hydrogen cyanide (HCN), also known as hydrocyanic acid, is a colorless gas or liquid with a boiling point of 25.7˚C, a vapor pressure of 100 kPa at 26˚C and Henry's Law constant of 6.4 atm/mole [4], this makes HCN very volatile.Thus, low pH, high temperature, low pressure, and intimate contact with air, all tend to increase the rate of dissipation of cyanide from solution as hydrogen cyanide.In addition to free cyanide, other complexes such as the metal cyanide complexes formed with gold, silver, copper, nickel, iron and cobalt must be considered.
In cyanidation plants all around the world, the concentration of cyanide used to dissolve gold in ores is typically higher than the stoichiometric ratio, due to the solubility of other minerals.Free cyanide produces complexes with several metallic species, especially transition metals, which show a broad variation in both stability and solubility.Many common copper minerals are soluble in the dilute cyanide solution under typical of leach conditions found in the gold cyanidation process.Minerals such as azurite and malacite, are rapidly leached and are soluble in dilute cyanide solutions.
Enargite and chalcopyrite leach more slowly but are sufficiently soluble to cause excessive cyanide loss and contamination of the pregnant leach solutions.In reactions in aqueous solutions the cupric ion is rapidly converted to cuprous form and then copper forms a series of extremely stable soluble complexes in cyanide such as: Under typical gold cyanidation conditions The high consumption of cyanide during the cyanidation of copper-gold ores is due to the fact that copper forms complexes of high coordination numbers with cyanide (Reaction 3 to 6), 3 in particular.Therefore, hydrometallurgical treatment of these ores by cyaniding as a rule gives rise to a series of difficulties associated with increase in the cyanide consumption and decrease in the dissolution rate of gold and silver, and in the cementation process.This precipitate is of low quality, because the copper is precipitated along with gold and silver, resulting in a higher consumption of zinc dust, fluxes in the smelting of the precipitate and shorter life for crucibles.
In this regard a study is proposed to remove copper cyanide ions with, a very promising electrochemical treatment technique, which does not require chemical additions.This process is electrocoagulation (EC).The EC process operates on the principle that coagulation of cop-per cyanide ions from barren solutions from the Merrill-Crowe process is caused by the combined effects of electrolysis gases (H 2 and O 2 ) and the electrolytic production of cations from the iron anodes that corrode during electrolysis.

Electrocoagulation Fundamentals he cations ipolar electrodes are us
The EC process operates on the principle that t produced electrolytically from iron and/or aluminum anodes enhance the coagulation of contaminants from an aqueous medium.Electrophoretic motion tends to concentrate negatively charged particles in the region of the anode and positively charged ions in the region of the cathode.The consumable, or sacrificial, metal anodes are used to continuously produce polyvalent metal cations in the vicinity of the anode.These cations neutralize the negative charge of the particles carried toward the anodes by electrophoretic motion, thereby facilitating coagulation.In the flowing EC techniques, the production of polyvalent cations from the oxidation of the sacrificial anodes (Fe and Al) and the electrolysis gases (H 2 and O 2 ) works in combination to flocculate the coagulant materials [6], the gas bubbles produced by the electrolysis carry the pollutant to the top of the solution where it is concentrated, collected and removed.Figure 2 illustrates the schematic diagram of the process.
Generally, in the EC process b ed.Pretorius [7] and Mameri [8] have reported on the use of cells with bipolar electrode arranged in series.These cells, operated at relatively low current densities, produce iron or aluminum coagulant in a more effective, fast and economical manner when compared to chemical coagulation.The savings result from a reduction in the time necessary for the treatment and an increase in the anodic area improved the efficiency of the electrolysis [7,8].An electrocoagulation cell with bipolar electrodes cted in series is shown in Figure 3.The inner trodes are bipolar, that is they carry both positive and negative charges on opposing faces.These charges develop on the electrode surfaces and are opposite in sign of the charge carried by the parallel electrode surface (refer to Figure 3).During electrolysis the positive side of these bipolar electrodes undergoes anodic reactions, while on the negative side, cathodic reactions occur.
The released ions neutralize the charge of the parti d thereby initiate coagulation.The bipolar arrangement reduces the time needed for the treatment due to the increase in surface area mentioned above.This arrangement also has the practical advantage of simplified set-up in that only two monopolar electrodes are connected to the electric power source with no interconnections between the inner bipolar electrodes.

Electrocoagulation Process
The chemicals reactions that have scribe the mechanism of EC for the production of H 2(g) and  

Fe OH F
      of these reactions in an EC ocess, using iron electrodes, is shown in Figure 4.As mentioned above, the gas bubbles produced by electrolysis carry the copper along with the sludge to the top of the solution where it is collected and removed [10].However, it is the reactions of the metal ions that enhance the formation of the coagulant.The metal cations are hydrolyzed, releasing hydrogen ions that in hydrogen evolution at the cathode, to yield both soluble and insoluble hydroxides that will react with or adsorb copper from the cyanide solution and also contribute to coagulation by neutralizing the negatively charged colloidal particles that may be present at neutral or alkaline pH.This enables the particles to approach closely and agglomerate under the influence of Van der Waals attracttive forces.The pH of the medium rises as a result of this electrochemical process and the Fe(OH) n(s) formed remains in the aqueous stream as gelatinous suspension, which can remove the

Cu CN
 from the barren solution, either by complexation or by electrostatic attraction followed of coagulation and flotation [11].Generally, in the EC process, bipolar electrodes are used.It has been reported that cells with bipolar electrodes, connected in series and operating at relatively low current densities [12], produce iron or aluminum coagulant more effecttively, more rapidly and more economically when compared to chemical coagulation.

Experimental Details
The experimental work was p solution from the Merrill Crowe process containing an average in the range of 660 -712 ppm of copper.EC experiments were performed using a 600 ml Pyrex beaker glass (Figure 5), equipped with two iron electrodes (10 cm × 2.5 cm) with an electrode separation of 5 mm.A regulated power supply (model Steren PRL-25) to provide the necessary energy to the electrocoagulation cell, magnetic stirrer (Model PC-310, Corning) with 100 rpm was used, and the initial and final pH was taken with a pH meter (VWR Scientific 8005), filtration was performed with Whatman filter paper No.42.To determine the adsorption copper in iron hydroxide species generated at the anode, a barren solution after the cementation process was used that was provided by the William Mine Co.This solution contained an average of 0.02 mg/L gold and 0.1 mg/L silver along with amounts of zinc, lead.Among others, the analysis was performed according to EPA 200.detection of metals and trace elements by ICP/atomic emission spectrometry).The solution and the solids were separated by filtration through filter paper, the sludge from the EC was dried for 8 hrs in an oven at 80˚C.The tables below show the initial conditions of the EC test to remove copper.

Optimization of Parameters
In order to find the optimum parameters of the EC process for the removal of copper, experiments were carried out by changing the pH of the solution, residence time in the EC cell and voltage and amperage.

Results
Tables 1-3 show the results for tests performed with 4 g or pH 8 and 4 g/liter of NaCl.
Sludge Chemical Essay rams/liter of sodium chloride.
From these results it was determined that the optimum parameters were: pH 8, residence time of 20 minutes and 4 grams/liter of NaCl, this achieved 99% copper removal.Also, when the time increased from 15 to 20 minutes the removal of copper increased from 92% to 99%, this occurs in the pH range from 8 to 9 approximately, this coincides with the production of the magnetic iron, Fe 3 O 4 , which has magnetic properties that accelerates the process of adsorption of metals, the adsorption rate is then physically, because it is caused by the magnetic forces of the magnetite into copper, without altering their chemical composition.This removal of copper also can explain with a decrease in the zeta potential on iron hydroxides which causes a decrease in repulsive forces between the particles, generated collision between particles thus favors the formation of flocs which float to the water surface through micro bubbles generated from oxygen and hy- drogen rom the iron electrodes.Also, the ad ages o the EC process is the decomposing of cyanide at the anode, re the an oxidatio cyanide is propo tional t the alkalinity of the electrolyte and consistent with the following anism: F ows tim tion w it is ob behavi pper.

Product Characterization
In order to identify the iron species present, Scanning Electron Microscope /EDX) w ed to ch rize the solid products ed during ocess for moval of copper with iron electrod aces of these iron oxide/ the EC pr es.re

Scanning Electron Microscopy (SEM/EDAX)
Figure 7 shows SEM image and Figure 8 shows EDAX of copper adsorbed on iron species.These SEM and EDAX results show that the surf oxyhydr particles were ted with a layer of copper.

X-Ray Diffraction
Diffract s were obtai with a Bruker XS D4 Endeavor diffractometer operating with a Cu-K radiation source filtered with a gr ite monochrom r (λ = 1.5406Å).The samples were wet ground to a fine pow-Sigma-Aldrich) and pressed into a sample holder.The XRD scans were recorded from 20˚ to h and with a 10 s c g ti st i rem im kV a ow 9, shows a diffractogram of the filtered solid products (the feed solution contained 700 ppm of copper and the pH of the solution after EC was ~10).
s figure indicates the presence of magnetite, geothite, iron hydroxi xide, and lepidocrocite in the solid pr cts.

Conclusions
Electrocoagulation process was carried out to obtain a 99% of copper removal.The optimal operations conditions were: pH = 8, residence time: 20 minutes and 4 g/l of sodium chloride as conductivity modifier.The solid product obtained from EC process was 13% copper and 24% iron.The EC process does not generate any smell in the process of elimination of copper from the barren solution.During the EC process is not necessary to add any reagent (except Nacl), since the coagulating agent is generated in situ.
We found that it is possible to reduce the copper cyanid in 20 minutes.
Also, the results of this study suggest that EC produces magnetic particles of magnetite.lepidocrocita and amorphous iron oxyhydroxide species that can be used to removal copper.The Scanning Electronic Microscopy, techniques demonstrate that the formed species are of magnetic type, like lepidocrocite and magnetite which adsorbed the copper particles on his surface due to the electrostatic attraction between both metals.

Figure 1 .
Figure 1.Equilibrium distribution diagram for cyanide as a function of pH.
to be the dominant species from the Eh-pH diagram for the copper-cyanide-water system[4,5].

Figure 2 .
Figure 2. Schematic diagram of the EC process

Figure 3 .
Figure 3.A schematic representation of a bipolar electrocoagulation cell and the equivalent electrical circuit (resistors reflects electrode surfaces).

Figure 4 .
Figure 4.An illustration of the EC mechanism (ar w indi-

Figure 5 .
Figure 5. EC schematic diagram of the experimental setup.